Synthesis, Characterization, and Electrochemical Properties of a Series of Sterically Varied Iron(II) Alkoxide Precursors and Their Resultant Nanoparticles
Timothy J. Boyle; Leigh Anna M. Ottley; Christopher A. Apblett; Constantine A. Stewart; Sarah M. Hoppe; Krista L. Hawthorne; Mark A. Rodriguez; Inorganic Chemistry 50 (2011) 6174–6182; doi:10.1021/ic200423m

data_4325493
_publ_section_title
;
 Synthesis, Characterization, and Electrochemical Properties of a Series
 of Sterically Varied Iron(II) Alkoxide Precursors and Their Resultant
 Nanoparticles
;
_journal_name_full               'Inorganic Chemistry'
_journal_page_first              6174
_journal_page_last               6182
_journal_paper_doi               10.1021/ic200423m
_journal_volume                  50
_journal_year                    2011
_chemical_formula_sum            'C46 H36 Fe N2 O2'
_chemical_formula_weight         704.62
_space_group_IT_number           14
_symmetry_cell_setting           monoclinic
_symmetry_space_group_name_Hall  '-P 2yn'
_symmetry_space_group_name_H-M   'P 1 21/n 1'
_atom_sites_solution_hydrogens   geom
_atom_sites_solution_primary     direct
_atom_sites_solution_secondary   difmap
_audit_creation_method           SHELXL-97
_cell_angle_alpha                90.00
_cell_angle_beta                 109.558(3)
_cell_angle_gamma                90.00
_cell_formula_units_Z            4
_cell_length_a                   13.131(2)
_cell_length_b                   15.622(3)
_cell_length_c                   19.182(4)
_cell_measurement_temperature    173(2)
_cell_volume                     3707.8(12)
_computing_cell_refinement       'Bruker SMART'
_computing_data_collection       'Bruker SMART'
_computing_data_reduction        'Bruker SAINT'
_computing_molecular_graphics    'Bruker SHELXTL'
_computing_publication_material  'Bruker SHELXTL'
_computing_structure_refinement  'SHELXL-97 (Sheldrick, 1997)'
_computing_structure_solution    'SHELXS-97 (Sheldrick, 1990)'
_diffrn_ambient_temperature      173(2)
_diffrn_measured_fraction_theta_full 0.999
_diffrn_measured_fraction_theta_max 0.999
_diffrn_measurement_device_type  'CCD area detector'
_diffrn_measurement_method       'phi and omega scans'
_diffrn_radiation_monochromator  graphite
_diffrn_radiation_source         'fine-focus sealed tube'
_diffrn_radiation_type           MoK\a
_diffrn_radiation_wavelength     0.71073
_diffrn_reflns_av_R_equivalents  0.0198
_diffrn_reflns_av_sigmaI/netI    0.0146
_diffrn_reflns_limit_h_max       14
_diffrn_reflns_limit_h_min       -14
_diffrn_reflns_limit_k_max       17
_diffrn_reflns_limit_k_min       -17
_diffrn_reflns_limit_l_max       21
_diffrn_reflns_limit_l_min       -21
_diffrn_reflns_number            22375
_diffrn_reflns_theta_full        23.27
_diffrn_reflns_theta_max         23.27
_diffrn_reflns_theta_min         2.10
_exptl_absorpt_coefficient_mu    0.447
_exptl_absorpt_correction_T_max  0.939
_exptl_absorpt_correction_T_min  0.923
_exptl_absorpt_correction_type   empirical
_exptl_absorpt_process_details   SADABS
_exptl_crystal_colour            yellow
_exptl_crystal_density_diffrn    1.262
_exptl_crystal_description       irregular
_exptl_crystal_F_000             1472
_exptl_crystal_size_max          0.20
_exptl_crystal_size_mid          0.15
_exptl_crystal_size_min          0.14
_refine_diff_density_max         0.247
_refine_diff_density_min         -0.154
_refine_diff_density_rms         0.036
_refine_ls_extinction_method     none
_refine_ls_goodness_of_fit_ref   1.031
_refine_ls_hydrogen_treatment    constr
_refine_ls_matrix_type           full
_refine_ls_number_parameters     460
_refine_ls_number_reflns         5337
_refine_ls_number_restraints     0
_refine_ls_restrained_S_all      1.031
_refine_ls_R_factor_all          0.0292
_refine_ls_R_factor_gt           0.0273
_refine_ls_shift/su_max          0.002
_refine_ls_shift/su_mean         0.000
_refine_ls_structure_factor_coef Fsqd
_refine_ls_weighting_details
'calc w=1/[\s^2^(Fo^2^)+(0.0437P)^2^+1.0570P] where P=(Fo^2^+2Fc^2^)/3'
_refine_ls_weighting_scheme      calc
_refine_ls_wR_factor_gt          0.0737
_refine_ls_wR_factor_ref         0.0753
_reflns_number_gt                4983
_reflns_number_total             5337
_reflns_threshold_expression     >2sigma(I)
_cod_data_source_file            ic200423m_si_001_07.cif
_cod_data_source_block           10fb161ss
_cod_original_cell_volume        3707.9(12)
_cod_database_code               4325493